Intersubband absorption properties of high Al content Al x Ga1−xN/GaN multiple quantum wells grown with different interlayers by metal organic chemical vapor deposition
© Sun et al.; licensee Springer. 2012
Received: 7 October 2012
Accepted: 19 November 2012
Published: 26 November 2012
High Al content Al x Ga1−xN/GaN multiple quantum well (MQW) films with different interlayers were grown by metal organic chemical vapor deposition. These MQWs were designed to achieve intersubband (ISB) absorption in the mid-infrared spectral range. We have considered two growth conditions, with AlGaN interlayer and GaN/AlN superlattice (SL) interlayer, both deposited on GaN-on-sapphire templates. Atomic force microscopy images show a relatively rough surface with atomic-step terraces and surface depression, mainly dominated by dislocations. High-resolution X-ray diffraction and transmission electron microscopy analyses indicate that good crystalline quality of the AlGaN/GaN MQW layer could be achieved when the AlGaN interlayer is inserted. The ISB absorption with a peak at 3.7 μm was demonstrated in MQW films with AlGaN interlayer. However, we have not observed the infrared absorption in MQW films with GaN/AlN SL interlayer. It is believed that the high dislocation density and weaker polarization that resulted from the rough interface are determinant factors of vanished ISB absorption for MQW films with the GaN/AlN SL interlayer.
KeywordsQuantum wells Interface Intersubband TEM PACS 61.72.Lk 61.05.cp 68.37.-d 61.72.uj
AlGaN/GaN multiple quantum well (MQW) structures grown on GaN/sapphire templates (GaN templates) have attracted much interest for intersubband (ISB) transition devices operating in the near-infrared and mid-infrared spectral ranges, such as photovoltaic and photoconductive GaN/AlN quantum well (QW) detectors and electrooptical modulators, benefiting from the large conduction-band offset (1.75 eV) between GaN and AlN. In addition, material transparency in a wide spectral region (360 nm to 13μm for GaN), large longitudinal-optical phonon energy (92 meV for GaN), and the rather heavy-electron effective mass (0.22 × m0 for GaN) also guarantee the realization of ISB transitions at room temperature. Short-wavelength ISB absorption has been reported by several groups in AlGaN/GaN MQW structures[4–7] and coupled QWs; ISB absorption at telecommunication wavelengths has also been observed at room temperature in self-organized GaN/AlN quantum dots[9, 10]. Until now, most of the progress was made by molecular beam epitaxy[11, 12], which is best suited for growing sharp QW interfaces in nitride-based ISB devices because of its inherently low growth temperature and slow growth rate. By contrast, metal organic chemical vapor deposition (MOCVD) is the most economically feasible technique for the mass production of such ISB devices. Although many papers have been published on AlGaN/GaN MQW films grown by MOCVD, ISB devices employing the AlGaN/GaN MQW structure grown by MOCVD are few[13, 14]. Therefore, further research and development by MOCVD are essential.
Obstacles still exist to hinder the development of AlGaN/GaN MQWs grown by MOCVD. There is a large lattice and thermal mismatch between the high Al content AlGaN/GaN MQW layer and the GaN templates. The biaxial tensile strain in the MQW layer accumulates in the process of the MQW layering, grows thicker, and finally leads to crack formation[15, 16]. Moreover, the tensile strain will induce a large density of threading dislocations[17, 18], a typical problem of III-nitride layers grown on foreign substrates (109 to 1010 cm−2). Additionally, the Al(Ga)N/GaN interface is found to be unstable when it is pseudomorphically strained onto GaN. The alloyed interface is formatted under stress, especially growing at high growth temperatures by MOCVD[19, 20]. This interface degradation in MQW structures affects the ISB absorptions. In order to overcome these problems, it is necessary to adopt some strain relaxation techniques for MQW structure growth.
In this paper, we inserted different interlayers in the MQW structure to solve these problems. High Al content Al0.4Ga0.6N/GaN MQW films were grown by MOCVD with different interlayers. The remainder of this paper is organized as follows. Initially, the detailed deposition process of the film growth is described, followed by the presentation of morphology, structures, and optical properties of MQW films. Finally, it provides the result that, with the insertion of different interlayers, MQW film strain relaxation differs. To get a good insight into the strain relaxation, we analyzed MQWs using different characterization techniques.
All samples were grown on (0001) sapphire substrates by Thomas Swan MOCVD system (Thomas Swan & Co., Ltd., County Durham, UK). A 2-μm-thick GaN template was first grown with H2 atmosphere. Samples consisted of 20 periods of Al0.4Ga0.6N/GaN MQW structures and a 10-nm Al0.4Ga0.6N cap layer. The thicknesses of the Al0.4Ga0.6N barrier and the GaN well were 5 and 3 nm in MQW structures, respectively. Si doping in the GaN well layer was conducted with SiH4 at a doping level of 6 × 1018 cm−3. In order to relax the stress, two sets of interlayer structures were designed and prepared. A 20-nm Al0.3Ga0.7N interlayer was inserted between the AlGaN/GaN MQW layer and the GaN template in sample A, whereas four periods of GaN/AlN superlattice (SL) layers (AlN barriers, 3.6 nm; GaN wells, 1.4 nm) were employed for sample B as the interlayer. The interlayer inserted in samples A and B was coherent with the MQW layer in design. Growth parameters were the same for the AlGaN/GaN MQW layer and the cap layer in different samples.
High-resolution X-ray diffraction (HRXRD) measurements were performed with Bede D1 high-resolution X-ray diffractometer (Bede X-ray Metrology, Durham, England, UK). ω-2θ Scan of the (0002) X-ray reflection, ω-scan for the symmetric (0002), and skew symmetric (10–12) reflections of MQW films were utilized to characterize the crystalline quality of AlGaN/GaN MQW layers. Surface morphology was characterized by Pico Scan TM 2500 (PicoPlus, Tempe, AZ, USA) atomic force microscopy (AFM). Microstructures were studied using a JEOL 2010F high-resolution transmission electron microscope (HRTEM) (JEOL Ltd., Akishima, Tokyo, Japan) operated at 200 kV. All TEM samples were prepared following the standard procedure of grinding, dimpling, and ion milling until electron transparency is achieved. ISB absorption was investigated using a Bruker 120HR Fourier transform infrared spectroscope (BRUKER AXS GMBH, Karlsruhe, Germany) with a single transmission of p-polarized light incident at the Brewster's angle at room temperature.
Results and discussion
Surface roughness and FWHM of ω -scan for (0002) and (10–12) reflections of samples A and B
where β m is the measured FWHM, β 0 is the intrinsic rocking curve width of the crystal, β d is the instrumental broadening width, β α is the broadening from lattice rotations at dislocations (tilt or twist), β ε is the broadening due to lattice strain at dislocations (often called microstrain), β L is the broadening due to limited correlation lengths, and β r is the broadening due to wafer curvature. For ω-scan of symmetric (0002) and asymmetric (10–12) reflections, the FWHM broadening of zero-order satellite peaks mainly come from β α . When the threading dislocation density is close to 109 cm−2, β L cannot be neglected. Furthermore, the interlayer in design is coherent with the MQW layer; the peak of interlayer and the MQW zero-order satellite peaks are overlapped in sample B, and the interlayer also contributes to the broadening of ω-scan. Therefore, the threading dislocation density of MQW films cannot be accessed directly by the FWHM of ω-scan.
In conclusion of Figure3, the stress induced by the interlayer changes the propagation of dislocations. In sample A, the inserted AlGaN interlayer thickness exceeds the critical thickness of elastic relaxation. The AlGaN interlayer was plastic relaxed, as proven by the difference of peak locations in Figure2. The tensile stress is strong enough to allow dislocations to meet, react, and annihilate. However, in sample B, the thickness of the GaN/AlN SL interlayer is the same as the AlGaN interlayer in sample A; the GaN/AlN SL interlayer is still under elastic relaxation, and the stress only makes dislocations inclined. Thus, dislocations incline and subsequently go into the MQW layer and finally make the dislocation density higher in sample B. Other stress relaxation paths are also present; cracks are shown in Figure1b. Therefore, stress influences the propagation of dislocations as different interlayers were inserted. Details of dislocation behavior were discussed in another work. From the results, it is manifested that the AlGaN interlayer effectively blocks the threading dislocation.
In sample B, threading dislocations entered the MQW layer, and no ISB absorption was presented in Figure4. The absence of ISB absorption can be attributed to those reasons as shown below. First, the high density of threading edge dislocations exists in sample B. It was discovered that edge dislocations in III-nitride cause propagation loss for transverse-magnetic (TM) polarization of light in a waveguide. Edge dislocations introduce acceptor centers along the dislocation lines, and electrons are captured by the acceptor centers. Eventually, charges perpendicularly align and work like a wire-grid polarizer. This excess polarization-dependent loss is critical for ISB since ISB occurs only for TM polarization in a waveguide structure. Second, polarization charge in the GaN/AlGaN heterostructure will surely influence ISB intensity since ISB absorption strongly relies on the net carrier density in the QW. Compositionally graded AlGaN films grown on unintentionally doped GaN templates can achieve high electron-sheet concentrations which are results of polarization-induced doping[27–29]. According to the HRXRD analysis, order satellite peaks at −1 were present in sample B. No higher-order peaks manifested the rough interface in the MQW layer. As is well known, the electron density is crucial to the infrared absorption property of the ISB devices because electron–hole pairs cannot be generated only in the conductive band. The rough interface of the sample with SL interlayer surely decreased polarization-induced net electron density in the quantum well. Besides, interface instability pushes the first excited electron state close to the barrier conduction band edge. As a consequence, the e1 and e2 oscillator strength is reduced, and the ISB absorption becomes weak or even vanishes.
In conclusion, high Al content AlGaN/GaN MQW films grown with different interlayers by metal organic chemical vapor deposition were investigated using AFM, HRXRD, and HRTEM. The MQW films present a relatively rough surface with atomic-step terraces and surface depression. Good crystalline quality of the AlGaN/GaN MQW layer could be obtained with the inserted AlGaN interlayer. The AlGaN interlayer under plastic stress effectively blocked the threading dislocation, but the GaN/AlN SL interlayer in the same thickness under elastic stress just inclined the threading dislocation. The ISB absorption with a peak at 3.7 μm in MQWs with the AlGaN interlayer, the high dislocation density, and the rough interface are the reasons of ISB absorption vanishing for MQW films with GaN/AlN SL interlayer.
Atomic force microscopy
Full width at half maximum
High-resolution transmission electron microscopy
High-resolution X-ray diffraction
Metal organic chemical vapor deposition
Multiple quantum wells
The authors thank Professor XD Han and Dr. LH Wang from the Institute of Microstructure and Properties of Advanced Materials in Beijing University of Technology for their help with the HRTEM experiment and Dr M Xiong for the useful discussion. This study is supported by the Heilongjiang Province's Nature Science Foundation of China (grant no: F2007-1) and the Open Experimentation Program of Beijing Institute of Technology (BJUT-GTS-200904).
- Hofstetter D, Baumann E, Giorgetta FR, Théron R, Wu H, Schaff WJ, Dawlaty J, George PA, Eastman LF, Rana F, Kandaswamy PK, Leconte S, Monroy E: Photodetectors based on intersubband transitions using III-nitride superlattice structures. J Phys-Condes Matter 2009, 21: 174218.View ArticleGoogle Scholar
- Baumann E, Giorgetta FR, Hofstetter D, Leconte S, Guillot F, Bellet-Amalric E, Monroy E: Electrically adjustable intersubband absorption of a GaN/AlN superlattice grown on a transistor like structure. Appl Phys Lett 2006, 89: 101121. 10.1063/1.2348759View ArticleGoogle Scholar
- Welna M, Kudrawiec R, Motyka M, Kucharski R, Zając M, Rudziński M, Misiewicz J, Doradziński R, Dwiliński R: Transparency of GaN substrates in the mid-infrared spectral range. Cryst Res Technol 2012, 47: 347–350. 10.1002/crat.201100443View ArticleGoogle Scholar
- Gmachl C, Ng HM, Chu SNG, Cho AY: Intersubband absorption at λ 1.55 μm in well- and modulation-doped GaN/AlGaN multiple quantum wells with superlattice barriers. Appl Phys Lett 2000, 77: 3722–3724. 10.1063/1.1332108View ArticleGoogle Scholar
- Kishino K, Kikuchi A, Kanazawa H, Tachibana T: Intersubband transition in (GaN)m/(AlN)n superlattices in the wavelength range from 1.08 to 1.61 μm. Appl Phys Lett 2002, 81: 1234–1236. 10.1063/1.1500432View ArticleGoogle Scholar
- Zhou QY, Chen JY, Pattada B, Manasreh MO, Xiu FX, Puntigan S, He L, Ramaiah KS, Morkoc H: Infrared optical absorbance of intersubband transitions in GaN/AlGaN multiple quantum well structures. J Appl Phys 2003, 93: 10140–10142. 10.1063/1.1577809View ArticleGoogle Scholar
- Kandaswamy PK, Guillot F, Bellet-Amalric E, Monroy E, Nevou L, Tchernycheva M, Michon A, Julien FH, Baumann E, Giorgetta FR, Hofstetter D, Remmele T, Albrecht M, Birner S, Dang LS: GaN/AlN short-period superlattices for intersubband optoelectronics: a systematic study of their epitaxial growth, design, and performance. J Appl Phys 2008, 104: 093501. 10.1063/1.3003507View ArticleGoogle Scholar
- Driscoll K, Liao YT, Bhattacharyya A, Zhou L, Smith DJ, Moustakas TD, Paiella R: Optically pumped intersubband emission of short-wave infrared radiation with GaN/AlN quantum wells. Appl Phys Lett 2009, 94: 081120. 10.1063/1.3089840View ArticleGoogle Scholar
- Moumanis K, Helman A, Fossard F, Tchernycheva M, Lusson A, Julien FH, Damilano B, Grandjean N, Massies J: Intraband absorptions in GaN/AlN quantum dots in the wavelength range of 1.27–2.4 μm. Appl Phys Lett 2003, 82: 868–870. 10.1063/1.1543238View ArticleGoogle Scholar
- Tchernycheva M, Nevou L, Doyennette L, Helman A, Colombelli R, Julien FH, Guillot F, Monroy E, Shibata T, Tanaka M: Intraband absorption of doped GaN/AlN quantum dots at telecommunication wavelengths. Appl Phys Lett 2005, 87: 101912–101913. 10.1063/1.2042540View ArticleGoogle Scholar
- Ng HM, Gmachl C, Chu SNG, Cho AY: Molecular beam epitaxy of GaN/AlxGa1−xN superlattices for 1.52–4.2 μm intersubband transitions. J Cryst Growth 2000, 220: 432–438. 10.1016/S0022-0248(00)00888-5View ArticleGoogle Scholar
- Machhadani H, Kandaswamy P, Sakr S, Vardi A, Wirtmüller A, Nevou L, Guillot F, Pozzovivo G, Tchernycheva M, Lupu A, Vivien L, Crozat P, Warde E, Bougerol C, Schacham S, Strasser G, Bahir G, Monroy E, Julien FH: GaN/AlGaN intersubband optoelectronic devices. New J Phys 2009, 11: 16.View ArticleGoogle Scholar
- Hoshino K, Someya T, Hirakawa K, Arakawa Y: Low-pressure MOCVD growth of GaN/AlGaN multiple quantum wells for intersubband transitions. J Cryst Growth 2002, 237: 1163–1166.View ArticleGoogle Scholar
- Péré-Laperne N, Bayram C, Nguyen-Thê L, McClintock R, Razeghi M: Tunability of intersubband absorption from 4.5 to 5.3 μm in a GaN/Al0.2Ga0.8N superlattices grown by metalorganic chemical vapor deposition. Appl Phys Lett 2009, 95: 131109. 10.1063/1.3242027View ArticleGoogle Scholar
- Einfeldt S, Heinke H, Kirchner V, Hommel D: Strain relaxation in AlGaN/GaN superlattices grown on GaN. J Appl Phys 2001, 89: 2160–2167. 10.1063/1.1342020View ArticleGoogle Scholar
- Kladko V, Kuchuk A, Lytvyn P, Yefanov O, Safriuk N, Belyaev A, Mazur YI, DeCuir EA Jr, Ware ME, Salamo GJ: Substrate effects on the strain relaxation in GaN/AlN short-period superlattices. Nanoscale Res Lett 2012, 7: 289. 10.1186/1556-276X-7-289View ArticleGoogle Scholar
- Moram MA, Ghedia CS, Rao DVS, Barnard JS, Zhang Y, Kappers MJ, Humphreys CJ: On the origin of threading dislocations in GaN films. J Appl Phys 2009, 106: 073513. 10.1063/1.3225920View ArticleGoogle Scholar
- Cherns PD, McAleese C, Kappers MJ, Humphreys CJ: Strain relaxation in an AlGaN/GaN quantum well system. In Springer Proceedings in Physics. Volume 120. Edited by: Cullis AG, Midgley PA. Berlin: Springer-Verlag; 2008:25–28.Google Scholar
- Boguslstrokawski P, Rapcewicz K, Bernholc JJ: Surface segregation and interface stability of AlN/GaN, GaN/InN, and AlN/InN 0001 epitaxial systems. Phys Rev B 2000, 61: 10820. 10.1103/PhysRevB.61.10820View ArticleGoogle Scholar
- Choi SC, Kim JH, Choi JY, Lee KJ, Lim KY, Yang GM: Al concentration control of epitaxial AlGaN alloys and interface control of GaN/AlGaN quantum well structures. J Appl Phys 2000, 87: 172–176. 10.1063/1.371840View ArticleGoogle Scholar
- Gong JR, Tseng SF, Huang CW, Tsai YL, Liao WT, Wang CL, Shi BH, Lin TY: Effects of Al-containing intermediate III-nitride strained multilayers on the threading dislocation density and optical properties of GaN films. Jpn J Appl Phys Part 1 - Regul Pap Short Notes Rev Pap 2003, 42: 6823–6826.View ArticleGoogle Scholar
- Kuwano N, Tsuruda T, Adachi Y, Terao S, Kamiyama S, Amano H, Akasaki I: Annihilation of threading dislocations in GaN/AlGaN. Phys Status Solidi A-Appl Res 2002, 192: 366–370. 10.1002/1521-396X(200208)192:2<366::AID-PSSA366>3.0.CO;2-6View ArticleGoogle Scholar
- Moram MA, Vickers ME: X-ray diffraction of III-nitrides. Rep Prog Phys 2009, 72: 036502. 10.1088/0034-4885/72/3/036502View ArticleGoogle Scholar
- Sun HH, Guo FY, Li DY, Wang L, Zhao DG, Zhao LC: Dislocation behavior in AlGaN/GaN multiple quantum-well films grown with different interlayers. Chin Phys Lett 2012, 29: 096101. 10.1088/0256-307X/29/9/096101View ArticleGoogle Scholar
- Iizuka N, Kaneko K, Suzuki N: Polarization dependent loss in III-nitride optical waveguides for telecommunication devices. J Appl Phys 2006, 99: 093107. 10.1063/1.2195422View ArticleGoogle Scholar
- Lee SM, Belkhir MA, Zhu XY, Lee YH, Hwang YG, Frauenheim T: Electronic structures of GaN edge dislocations. Phys Rev B 2000, 61: 16033–16039. 10.1103/PhysRevB.61.16033View ArticleGoogle Scholar
- Li SB, Ware ME, Wu J, Minor P, Wang ZM, Wu ZM, Jiang YD, Salamo GJ: Polarization induced pn-junction without dopant in graded AlGaN coherently strained on GaN. Appl Phys Lett 2012, 101: 122103. 10.1063/1.4753993View ArticleGoogle Scholar
- Li SB, Ware ME, Wu J, Kunets VP, Hawkridge M, Minor P, Wang ZM, Wu ZM, Jiang YD, Salamo GJ: Polarization doping: reservoir effects of the substrate in AlGaN graded layers. J Appl Phys 2012, 112: 053711. 10.1063/1.4750039View ArticleGoogle Scholar
- Xu PQ, Jiang Y, Chen Y, Ma ZG, Wang XL, Deng Z, Li Y, Jia HQ, Wang WX, Chen H: Analyses of 2-DEG characteristics in GaN HEMT with AlN/GaN super-lattice as barrier layer grown by MOCVD. Nanoscale Res Lett 2012, 7: 141. 10.1186/1556-276X-7-141View ArticleGoogle Scholar
- Nicolay S, Feltin E, Carlin JF, Grandjean N, Nevou L, Julien FH, Schmidbauer M, Remmele T, Albrecht M: Strain-induced interface instability in GaN/AlN multiple quantum wells. Appl Phys Lett 2007, 91: 061927. 10.1063/1.2769399View ArticleGoogle Scholar
This article is published under license to BioMed Central Ltd. This is an Open Access article distributed under the terms of the Creative Commons Attribution License (http://creativecommons.org/licenses/by/2.0), which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.